Nokia Li-ion battery for powering a mobile phone
|Specific energy||(0.36–0.95 MJ/kg)|
|Energy density||(0.90–2.23 MJ/L)|
|Specific power||~250-~340 W/kg|
|Self-discharge rate||8% at 21 °C
15% at 40 °C
31% at 60 °C
|Nominal cell voltage||NMC 3.6 / 3.7 V, LiFePO4 3.2 V|
A lithium-ion battery (sometimes Li-ion battery or LIB) is a member of a family of rechargeable battery types in which lithium ions move from the negative electrode to the positive electrode during discharge and back when charging. Li-ion batteries use an intercalated lithium compound as the electrode material, compared to the metallic lithium used in non-rechargeable lithium battery.
Lithium-ion batteries are common in consumer electronics. They are one of the most popular types of rechargeable battery for portable electronics, with one of the best energy densities, no memory effect (note, however, that new studies have shown signs of memory effect in lithium-ion batteries), and only a slow loss of charge when not in use. Beyond consumer electronics, LIBs are also growing in popularity for military, electric vehicle and aerospace applications. For example, Lithium-ion batteries are becoming a common replacement for the lead acid batteries that have been used historically for golf carts and utility vehicles. Instead of heavy lead plates and acid electrolyte, the trend is to use a lightweight lithium/carbon negative electrodes and lithium iron phosphate positive electrodes. Lithium-ion batteries can provide the same voltage as lead-acid batteries, so no modification to the vehicle's drive system is required.
Chemistry, performance, cost and safety characteristics vary across LIB types. Handheld electronics mostly use LIBs based on lithium cobalt oxide (LiCoO
2), which offers high energy density, but presents safety risks, especially when damaged. Lithium iron phosphate (LFP), lithium manganese oxide (LMO) and lithium nickel manganese cobalt oxide (NMC) offer lower energy density, but longer lives and inherent safety. Such batteries are widely used for electric tools, medical equipment and other roles. NMC in particular is a leading contender for automotive applications. Lithium nickel cobalt aluminum oxide (NCA) and lithium titanate (LTO) are specialty designs aimed at particular niche roles.
Lithium-ion batteries can be dangerous under some conditions and can pose a safety hazard since they contain, unlike other rechargeable batteries, a flammable electrolyte and are also kept pressurized. Because of this the testing standards for these batteries are more stringent than those for acid-electrolyte batteries, requiring both a broader range of test conditions and additional battery-specific tests. This is in response to reported accidents and failures, and there have been battery-related recalls by some companies.
- 1 History
- 2 Construction
- 3 Electrochemistry
- 4 Charge and discharge
- 5 Production
- 6 Specifications
- 7 Materials of commercial cells
- 8 Uses
- 9 Self-discharge
- 10 Battery life
- 11 Safety
- 12 Research
- 12.1 Solid-state design (no electrolyte)
- 12.2 Tin electrode
- 12.3 Higher lithium content electrode
- 12.4 Silicon anode
- 12.5 Silicon-carbon anode
- 12.6 Sticky liquid electrolyte
- 12.7 Disorder in battery materials
- 12.8 Flexibility
- 12.9 Nonflammable perfluoropolyether electrolyte
- 12.10 Germanium nanowire-based anode
- 12.11 Uniformity of li-ions into and out of cathode
- 12.12 Architecture and controlling algorithm
- 12.13 Lithium iron phosphate cathode
- 12.14 Single-walled carbon nanotubes
- 12.15 Analysis of cathode
- 13 See also
- 14 References
- 15 Bibliography
- 16 External links
Before commercial introduction
Lithium batteries were first proposed by M. S. Whittingham, now at Binghamton University, while working for Exxon in the 1970s. Whittingham used titanium(IV) sulfide and lithium metal as the electrodes.
Reversible intercalation in graphite and intercalation into cathodic oxides was discovered in the 1970s by J. O. Besenhard at TU Munich. Besenhard proposed its application in lithium cells. Electrolyte decomposition and solvent co-intercalation into graphite were severe early drawbacks for battery life.
Primary lithium batteries with metallic lithium negative electrodes pose safety issues. As a result, lithium-ion batteries were developed in which both electrodes are made of a material containing lithium ions.[clarification needed]
At Oxford University, England, in 1979, John Goodenough and Koichi Mizushima demonstrated a rechargeable cell with voltage in the 4 V range using lithium cobalt oxide (LiCoO
2) as the positive electrode and lithium metal as the negative electrode.[clarification needed] This innovation provided the positive electrode material that made LIBs possible. LiCoO
2 is a stable positive electrode material which acts as a donor of lithium ions, which means that it can be used with a negative electrode material other than lithium metal. By enabling the use of stable and easy-to-handle negative electrode materials, LiCoO
2 opened a whole new range of possibilities for novel rechargeable battery systems.
In 1977, Samar Basu demonstrated electrochemical intercalation of lithium in graphite at the University of Pennsylvania. This led to the development of a workable lithium intercalated graphite electrode at Bell Labs (LiC
6) to provide an alternative to the lithium metal electrode battery.
In 1980, Rachid Yazami demonstrated the reversible electrochemical intercalation of lithium in graphite. The organic electrolytes available at the time would decompose during charging with a graphite negative electrode, slowing the development of a rechargeable lithium/graphite battery. Yazami used a solid electrolyte to demonstrate that lithium could be reversibly intercalated in graphite through an electrochemical mechanism. The graphite electrode discovered by Yazami is currently (2011-03-20) the most commonly used electrode in commercial lithium ion batteries.
In 1983, Michael M. Thackeray, Goodenough, and coworkers identified manganese spinel as a positive electrode material. Spinel showed great promise, given its low-cost, good electronic and lithium ion conductivity, and three-dimensional structure, which gives it good structural stability. Although pure manganese spinel fades with cycling, this can be overcome with chemical modification of the material. As of 2013 manganese spinel was used in commercial cells.
In 1985, Akira Yoshino assembled a prototype cell using carbonaceous material into which lithium ions could be inserted as one electrode, and lithium cobalt oxide (LiCoO
2), which is stable in air, as the other. By using materials without metallic lithium, safety was dramatically improved. LiCoO
2 enabled industrial-scale production and represents the birth of the current lithium-ion battery.
In 1989, Goodenough and Arumugam Manthiram of the University of Texas at Austin showed that positive electrodes containing polyanions, e.g., sulfates, produce higher voltages than oxides due to the induction effect of the polyanion.
From commercial introduction
The performance and capacity of lithium-ion batteries increases as development progresses.
In 1996 Goodenough, Akshaya Padhi and coworkers proposed lithium iron phosphate (LiFePO
4) and other phospho-olivines (lithium metal phosphates with the same structure as mineral olivine) as positive electrode materials.
In 2002 Yet-Ming Chiang and his group at MIT showed a substantial improvement in the performance of lithium batteries by boosting the material's conductivity by doping it with aluminium, niobium and zirconium. The exact mechanism causing the increase became the subject of widespread debate.
In 2004 Chiang again increased performance by utilizing iron phosphate particles of less than 100 nanometers in diameter. This decreased particle density almost one hundredfold, increased the positive electrode's surface area and improved capacity and performance. Commercialization led to a rapid growth in the market for higher capacity LIBs, as well as a patent infringement battle between Chiang and Goodenough.
As of 2011, lithium-ion batteries accounted for 66% of all portable secondary (i.e., rechargeable) battery sales in Japan.
By 2013 the lithium rechargeable battery had progressed to a lithium vanadium phosphate battery to increase energy efficiency in the forward and reverse reaction.
In 2014 John Goodenough, Yoshio Nishi, Rachid Yazami and Akira Yoshino were rewarded by The National Academy of Engineering for pioneering and leading the groundwork for today’s lithium ion battery. The prize, which is in its 25th year, includes a $500,000 award.
In 2014 batteries stated to have 20% higher capacity than those previously available, with a silicon anode rather than graphite (carbon) anode, were being delivered to smartphone manufacturers.
The three primary functional components of a lithium-ion battery are the positive and negative electrodes and electrolyte. Generally, the negative electrode of a conventional lithium-ion cell is made from carbon. The positive electrode is a metal oxide, and the electrolyte is a lithium salt in an organic solvent. The electrochemical roles of the electrodes reverse between anode and cathode, depending on the direction of current flow through the cell.
The most commercially popular negative electrode is graphite. The positive electrode is generally one of three materials: a layered oxide (such as lithium cobalt oxide), a polyanion (such as lithium iron phosphate) or a spinel (such as lithium manganese oxide).
The electrolyte is typically a mixture of organic carbonates such as ethylene carbonate or diethyl carbonate containing complexes of lithium ions. These non-aqueous electrolytes generally use non-coordinating anion salts such as lithium hexafluorophosphate (LiPF
6), lithium hexafluoroarsenate monohydrate (LiAsF
6), lithium perchlorate (LiClO
4), lithium tetrafluoroborate (LiBF
4) and lithium triflate (LiCF
Depending on materials choices, the voltage, energy density, life and safety of a lithium-ion battery can change dramatically. Recently, novel architectures using nanotechnology have been employed to improve performance.
Pure lithium is highly reactive. It reacts vigorously with water to form lithium hydroxide and hydrogen gas. Thus, a non-aqueous electrolyte is typically used, and a sealed container rigidly excludes moisture from the battery pack.
Lithium ion batteries are more expensive than NiCd batteries but operate over a wider temperature range with higher energy densities. They require a protective circuit to limit peak voltage.
For notebooks or laptops, lithium-ion cells are supplied as part of a battery pack with temperature sensors, voltage converter/regulator circuit, voltage tap, battery charge state monitor and the main connector. These components monitor the state of charge and current in and out of each cell, capacities of each individual cell (drastic change can lead to reverse polarities which is dangerous), temperature of each cell and minimize the risk of short circuits.
- Small cylindrical (solid body without terminals, such as those used in laptop batteries)
- Large cylindrical (solid body with large threaded terminals)
- Pouch (soft, flat body, such as those used in cell phones)
- Prismatic (semi-hard plastic case with large threaded terminals, such as vehicles' traction packs)
The absence of a case gives pouch cells the highest energy density; however, batteries using pouch and prismatic cells require an external means of containment to prevent expansion when their state-of-charge (SOC) level is high.
The participants in the electrochemical reactions in a lithium-ion battery are the negative and positive electrodes with the electrolyte providing a conductive medium for Lithium-ions to move between the electrodes.
Both electrodes allow lithium ions to move in and out of their interiors. During insertion (or intercalation) ions move into the electrode. During the reverse process, extraction (or deintercalation), ions move back out. When a lithium-ion based cell is discharging, the positive Lithium ion moves from the negative electrode (usually graphite) and enters the positive electrode (lithium containing compound). When the cell is charging, the reverse occurs.
The negative electrode half reaction is:
In a lithium-ion battery the lithium ions are transported to and from the positive or negative electrodes by oxidizing the transition metal, cobalt (Co), in Li
2 from Co3+
during charge, and reduced from Co4+
during discharge. The cobalt electrode reaction is only reversible for x < 0.5, limiting the depth of discharge allowable. This chemistry was used in the Li-ion cells developed by Sony in 1990.
The cell's energy is equal to the voltage times the charge. Each gram of lithium represents Faraday's constant/6.941 or 13,901 coulombs. At 3 V, this gives 41.7 kJ per gram of lithium, or 11.6 kWh per kg. This is a bit more than the heat of combustion of gasoline, but does not consider the other materials that go into a lithium battery and that make lithium batteries many times heavier per unit of energy.
The cell voltages given in the Electrochemistry section are larger than the potential at which aqueous solutions will electrolyze. Given lithium metal's high reactivity to water, nonaqueous or aprotic solutions are used.
Liquid electrolytes in lithium-ion batteries consist of lithium salts, such as LiPF
4 or LiClO
4 in an organic solvent, such as ethylene carbonate, dimethyl carbonate, and diethyl carbonate. A liquid electrolyte acts as a carrier between the positive and negative electrodes when current flows through an external circuit. Typical conductivities of liquid electrolyte at room temperature (20 °C (68 °F)) are in the range of 10 mS/cm (1 S/m), increasing by approximately 30–40% at 40 °C (104 °F) and decreasing slightly at 0 °C (32 °F).
Organic solvents easily decompose on the negative electrodes during charge. When appropriate organic solvents are used as the electrolyte, the solvent decomposes on initial charging and forms a solid layer called the solid electrolyte interphase (SEI), which is electrically insulating yet provides significant ionic conductivity. The interphase prevents further decomposition of the electrolyte after the second charge. For example, ethylene carbonate is decomposed at a relatively high voltage, 0.7 V vs. lithium, and forms a dense and stable interface.
Composite electrolytes based on POE (poly(oxyethylene)) developed by Syzdek et al., provide a relatively stable interface. It can be either solid (high molecular weight) and be applied in dry Li-polymer cells, or liquid (low molecular weight) and be applied in regular Li-ion cells.
Charge and discharge
During charging, an external electrical power source (the charging circuit) applies an over-voltage (a higher voltage but of the same polarity) than that produced by the battery, forcing the current to pass in the reverse direction. The lithium ions then migrate from the positive to the negative electrode, where they become embedded in the porous electrode material in a process known as intercalation.
The charging procedures for single Li-ion cells, and complete Li-ion batteries, are slightly different.
- A single Li-ion cell is charged in two stages:
- A Li-ion battery (a set of Li-ion cells in series) is charged in three stages:
During the constant current phase, the charger applies a constant current to the battery at a steadily increasing voltage, until the voltage limit per cell is reached.
During the balance phase, the charger reduces the charging current (or cycle the charging on and off to reduce the average current) while the state of charge of individual cells is brought to the same level by a balancing circuit, until the battery is balanced. Some fast chargers skip this stage. Some chargers accomplish the balance by charging each cell independently.
During the constant voltage phase, the charger applies a voltage equal to the maximum cell voltage times the number of cells in series to the battery, as the current gradually declines towards 0, until the current is below a set threshold of about 3% of initial constant charge current.
Periodic topping charge about once per 500 hours. Top charging is recommended to be initiated when voltage goes below 4.05 V/cell.
Lithium-ion is charged at approximately 4.2 ± 0.05 V/cell except for "military long life" that uses 3.92 V to extend battery life. Most protection circuits cut off if voltage greater than 4.3 V or temperature greater than 90 °C is reached. Below 2.50 V/cell the battery protection circuit may render the battery unchargeable with regular charging equipment. Most battery circuits stop at 2.7–3.0 V/cell.
Failure to follow current and voltage limitations can result in an explosion.
Charging at high and low temperatures
Charging temperature limits for Li-ion are stricter than operational limits. Lithium-ion performs well at elevated temperatures; however, prolonged exposure to heat reduces longevity.
Li‑ion batteries offer reasonably good charging performance at cooler temperatures and allow fast-charging in a temperature bandwidth of 5 to citation needed] (41 to 113 °F). Charging should be performed within this temperature range. At temperatures from 0 to 5 °C charging is possible, but the charge current should be reduced. During low-temperature charge the slight temperature rise above ambient due to the internal cell resistance is beneficial. Higher temperatures during charging may lead to battery degradation while charging at temperatures above 45 °C will degrade battery performance, whereas at lower temperatures the internal resistance of the battery will increase, resulting in less charging and longer charging times.[
Consumer-grade lithium-ion batteries cannot be charged at temperatures below 0 °C (32 °F). Although the pack appears to be charging normally, permanent plating of metallic lithium can occur on the anode during a subfreezing charge, and cannot be removed with cycling. Batteries with lithium plating are known to be more vulnerable to failure if exposed to vibration or other stressful conditions. Most devices equipped with Li-ion batteries do not allow charging outside of 0-45 °C for safety reasons, except for mobile phones that allow some degree of charging when they detect an emergency call in progress.
Industry produced about 660 million cylindrical lithium-ion cells in 2012; the 18650 format is by far the most popular for cylindrical cells. If Tesla meets its goal of shipping 40,000 Model S electric cars in 2014 and if the 85-kWh battery, which uses 7,000 of these cells, proves as popular overseas as it was in the U.S., in 2014 the Model S alone would use almost 40 percent of global cylindrical battery production. Production is gradually shifting to higher-capacity 3,000+ mAh cells. Annual flat polymer cell demand was expected to exceed 700 million in 2013.
- Specific energy density: 100 to 250 W·h/kg (360 to 900 kJ/kg)
- Volumetric energy density: 250 to 620 W·h/L (900 to 1900 J/cm³)
- Specific power density: 300 to 1500 W/kg (@ 20 seconds and 285 W·h/l)[not in citation given]
Because lithium-ion batteries can have a variety of positive and negative electrode materials, the energy density and voltage vary accordingly.
The open circuit voltage is higher than aqueous batteries (such as lead acid, nickel-metal hydride and nickel-cadmium). The internal resistance of widely used LiCoO
2 batteries is higher than that of nickel-metal hydride, nickel-cadmium, LiFePO
4 and lithium-polymer cells. Internal resistance increases with both cycling and age. Rising internal resistance causes the voltage at the terminals to drop under load, which reduces the maximum current draw. Eventually increasing resistance means that the battery can no longer operate for an adequate period.
Batteries with a lithium iron phosphate positive and graphite negative electrodes have a nominal open-circuit voltage of 3.2 V and a typical charging voltage of 3.6 V. Lithium nickel manganese cobalt (NMC) oxide positives with graphite negatives have a 3.7 V nominal voltage with a 4.2 V maximum while charging. The charging procedure is performed at constant voltage with current-limiting circuitry (i.e., charging with constant current until a voltage of 4.2 V is reached in the cell and continuing with a constant voltage applied until the current drops close to zero). Typically, the charge is terminated at 3% of the initial charge current. In the past, lithium-ion batteries could not be fast-charged and needed at least two hours to fully charge. Current-generation cells can be fully charged in 45 minutes or less and some types can reach 90% of full charge in as little as 10 minutes.
Materials of commercial cells
The increasing demand for batteries has led vendors and academics to focus on improving the energy density, operating temperature, safety, durability, charging time, output power, and cost of lithium ion battery solutions. The following materials have been used in commercially available cells. Research into other materials continues.
|Lithium Nickel Manganese Cobalt Oxide ("NMC", LiNixMnyCozO2)||Imara Corporation, Nissan Motor, Microvast Inc.||2008||density, output, safety|
|Lithium Manganese Oxide ("LMO", LiMn2O4)||Lucky Goldstar Chemical, NEC, Samsung, Hitachi, Nissan/AESC, EnerDel||Hybrid electric vehicle, cell phone, laptop||1996||durability, cost|
|Lithium Iron Phosphate ("LFP", LiFePO4)||University of Texas/Hydro-Québec, Phostech Lithium Inc., Valence Technology, A123Systems/MIT||Segway Personal Transporter, power tools, aviation products, automotive hybrid systems, PHEV conversions||1996||moderate density (2 A·h outputs 70 amperes) operating temperature >60 °C (140 °F)|
|Oxygen ("Li-Air")||IBM, Polyplus||Automotive||2012||Energy density: up to 10,000 mA·h per gram of positive electrode material. Rechargeable.|
|Graphite||The dominant negative electrode material used in lithium ion batteries.||1991||Low cost and good energy density|
|Lithium Titanate ("LTO", Li4Ti5O12)||9,000||Toshiba, Altairnano||automotive (Phoenix Motorcars), electrical grid (PJM Interconnection Regional Transmission Organization control area, United States Department of Defense), bus (Proterra)||2008||output, charging time, durability (safety, operating temperature −50–70 °C (−58–158 °F))[dead link]|
|Hard Carbon||Energ2||Consumer electronics||2013||greater storage capacity|
|Tin/Cobalt Alloy||Sony||Consumer electronics (Sony Nexelion battery)||2005||Larger capacity than a cell with graphite (3.5Ah 18650-type battery)|
|Silicon/Carbon||Volumetric: 580 W·h/l||Amprius||Smartphones, providing 1850 mA·h capacity||2013||Uses silicon and other electrochemicals. Energy density|
Li-ion batteries provide lightweight, high energy density power sources for a variety of devices. To power larger devices, such as electric cars, connecting many small batteries in a parallel circuit is more effective and more efficient than connecting a single large battery. Such devices include:
- Portable devices: these include mobile phones and smartphones, laptops and tablets, digital cameras and camcorders, electronic cigarettes, handheld game consoles and torches (flashlights).
- Power tools: Li-ion batteries are used in tools such as cordless drills, sanders, saws and a variety of garden equipment including whipper-snippers and hedge trimmers.
- Electric vehicles: Because of their light weight Li-ion batteries are used for energy storage for many electric vehicles for everything from electric cars to Pedelecs, from hybrid vehicles to advanced electric wheelchairs, from radio-controlled models and model aircraft to the Mars Curiosity rover.
Li-ion batteries are used in telecommunications applications. Secondary non-aqueous lithium batteries provide reliable backup power to load equipment located in a network environment of a typical telecommunications service provider. Li-ion batteries compliant with specific technical criteria are recommended for deployment in the Outside Plant (OSP) at locations such as Controlled Environmental Vaults (CEVs), Electronic Equipment Enclosures (EEEs), and huts, and in uncontrolled structures such as cabinets. In such applications, li-ion battery users require detailed, battery-specific hazardous material information, plus appropriate fire-fighting procedures, to meet regulatory requirements and to protect employees and surrounding equipment.
Batteries gradually self-discharge even if not connected and delivering current. Li+ rechargeable batteries have a self-discharge rate typically stated by manufacturers to be 1.5-2% per month. The rate increases with temperature and state of charge. A 2004 study found that for most cycling conditions self-discharge was primarily time-dependent; however, after several months of stand on open circuit or float charge, state-of-charge dependent losses became significant. The self-discharge rate did not increase monotonically with state-of-charge, but dropped somewhat at intermediate states of charge. Self-discharge rates may increase as batteries age.
For comparison, the self-discharge rate is over 30% per month for common nickel metal hydride (NiMH) batteries, dropping to about 1.25% per month for low self-discharge NiMH batteries, and 10% per month in nickel-cadmium batteries.
Rechargeable battery life is often stated in number of charge cycles, but depth of discharge is usually not explicitly stated. Apple Inc. clarify that a charge cycle means using all the battery's capacity, but not necessarily by full charge and discharge; e.g., using half the charge of a fully charged battery, charging it, and then using the same amount of charge again count as a single charge cycle.
It is widely stated on Web sites and other sources, without citing any evidence or source, that "lithium-ion batteries deteriorate over time, whether they're being used or not. So a spare battery won't last much longer than the one in use." However, manufacturers' information clearly indicates that the life of a battery that is not abused depends upon the number of charge cycles it undergoes, specifying typical battery capacity in terms of number of cycles (e.g., capacity dropping linearly to 80% over 500 cycles), with no mention of age of the battery. Battery performance is rarely specified over more than 500 cycles. This means that batteries of mobile phones, or other hand-held devices in daily use, are not expected to last longer than three years. But it is also quite possible to obtain lithium-ion batteries based on carbon anodes with more than 10.000 cycles.
All rechargeable batteries degrade with use, the capacity decreasing until it is unusably small. Li+ batteries last longer[unreliable source?][dubious ] if not deeply discharged (depleted) before recharging.
Batteries may last longer if not stored fully discharged. As the battery self-discharges over time, its voltage gradually reduces. When depleted below the low-voltage threshold of the protection circuit (2.4 to 2.9 V/cell, depending on chemistry) it will be disabled and cannot be further discharged until recharged. This because as the discharge progresses, the metallic contents of the cell are plated onto its internal structure creating an unwanted discharge path. It is recommended to store batteries at 40% charge level.[dubious ]
The rate of degradation of lithium-ion batteries is strongly temperature-dependent; they degrade much faster if stored or used at higher temperatures. The carbon negative electrode of the cell also generates heat. High charge levels and elevated temperatures (whether from charging or ambient air) hasten capacity loss. Poor ventilation may increase temperatures, further shortening battery life. Loss rates vary by temperature: 6% loss at 0 °C (32 °F), 20% at 25 °C (77 °F), and 35% at 40 °C (104 °F). In contrast, the calendar life of LiFePO
4 cells is not affected by high charge states. They may be stored in a refrigerator.
Charging forms deposits inside the electrolyte that inhibit ion transport. The increase in internal resistance reduces the cell's ability to deliver current. This problem is more pronounced in high-current applications. Older batteries also do not charge as much as new ones (charging time required decreases).
The need to "condition" NiCd and NiMH batteries has incorrectly leaked into folklore surrounding Li-ion batteries. The recommendation for the older technologies is to leave the device plugged in for seven or eight hours, even if fully charged. This may be a confusion of battery software calibration instructions with the "conditioning" instructions for NiCd and NiMH batteries. The software of a typical smart phone, for example, learns how to accurately gauge the battery's life by watching it discharge and leaving it on the charger produces a series of "micro discharges" that the software can watch and learn from.
Li-ion batteries require a battery management system to prevent operation outside each cell's safe operating area (over-charge, under-charge, safe temperature range) and to balance cells to eliminate state of charge mismatches, thereby significantly improving battery efficiency and increasing overall capacity. As the number of cells and load currents increase, the potential for mismatch increases. The two kinds of mismatch are state-of-charge (SOC) and capacity/energy ("C/E"). Though SOC is more common, each problem limits pack charge capacity (mA·h) to that of the weakest cell.
If overheated or overcharged, Li-ion batteries may suffer thermal runaway and cell rupture. In extreme cases this can lead to combustion. To reduce these risks, lithium-ion battery packs contain fail-safe circuitry that shuts down the battery when its voltage is outside the safe range of 3–4.2 V per cell. When stored for long periods the small current draw of the protection circuitry may drain the battery below its shutdown voltage; normal chargers are then ineffective. Many types of lithium-ion cells cannot be charged safely below 0 °C.
Other safety features are required in each cell:
- Shut-down separator (for overheating)
- Tear-away tab (for internal pressure)
- Vent (pressure relief)
- Thermal interrupt (overcurrent/overcharging)
These devices occupy useful space inside the cells, add additional points of failure and irreversibly disable the cell when activated. They are required because the negative electrode produces heat during use, while the positive electrode may produce oxygen. These devices and improved electrode designs reduce/eliminate the risk of fire or explosion. Further, these features increase costs compared to nickel metal hydride batteries, which require only a hydrogen/oxygen recombination device (preventing damage due to mild overcharging) and a back-up pressure valve. Contaminants inside the cells can defeat these safety devices.[clarification needed]
Short-circuiting a battery will cause the cell to overheat and possibly to catch fire. Adjacent cells may then overheat and fail, possibly causing the entire battery to ignite or rupture. In the event of a fire, the device may emit dense irritating smoke. The fire energy content (electrical + chemical) of cobalt-oxide cells is about 100 to 150 kJ per A·h, most of it chemical. Extinguishing this fire is dangerous as lithium burns violently when it comes in contact with water or moisture in the air; a suitable waterless fire extinguisher is recommended.
Replacing the lithium cobalt oxide positive electrode material in lithium-ion batteries with a lithium metal phosphate such as lithium iron phosphate improves cycle counts, shelf life and safety, but lowers capacity. As of 2006 these 'safer' lithium-ion batteries were mainly used in electric cars and other large-capacity battery applications, where safety is critical.
Lithium-ion batteries, unlike other rechargeable batteries, have a potentially hazardous pressurised flammable electrolyte, and require strict quality control during manufacture. A faulty battery can cause a serious fire. Faulty chargers can affect the safety of the battery because they can destroy the battery's protection circuit. While charging at temperatures below 0 °C, the negative electrode of the cells gets plated with pure lithium, which can compromise the safety of the whole pack. Battery packs which are not branded by a reputable manufacturer may not be built to the same safety standard as branded ones.
While fire is often serious, it may be catastrophically so. In about 2010 large lithium-ion batteries were introduced in place of other chemistries to power systems on some aircraft; as of January 2014[update] there had been at least four serious lithium-ion battery fires, or smoke, on the Boeing 787 passenger aircraft, introduced in 2011, which did not cause crashes but had the potential to do so.
Environmental concerns and recycling
Since Li-ion batteries contain no toxic metals (unlike other types of batteries which may contain lead or cadmium) they are generally categorized as non-hazardous waste. Li-ion battery elements including iron, copper, nickel and cobalt are considered safe for incinerators and landfills. These metals can be recycled, but mining generally remains cheaper than recycling. At present, not much is invested into recycling Li-ion batteries due to costs, complexities and low yield. The most expensive metal involved in the construction of the cell is cobalt. Lithium iron phosphate is cheaper but has other drawbacks. Lithium is less expensive than other metals used. The manufacturing processes of nickel and cobalt for the positive electrode and also the solvent, present potential environmental and health hazards.
In December 2006 Dell recalled approximately 22,000 laptop computer batteries. Approximately 10 million Sony batteries used in Dell, Sony, Apple, Lenovo, Panasonic, Toshiba, Hitachi, Fujitsu and Sharp laptops were recalled in 2006. The batteries were found to be susceptible to internal contamination by metal particles during manufacture. Under some circumstances, these particles could pierce the separator, causing a dangerous short-circuit.
In March 2007 computer manufacturer Lenovo recalled approximately 205,000 batteries at risk of explosion. In August 2007 mobile phone manufacturer Nokia recalled over 46 million batteries at risk of overheating and exploding. One such incident occurred in the Philippines involving a Nokia N91, which used the BL-5C battery.
IATA estimates that over a billion lithium cells are flown each year. The United States Department of Transportation has not allowed passengers on commercial aircraft to carry spare lithium batteries (i.e., not installed in a device) in their checked baggage since 1 January 2008. Types of batteries covered by this rule are those containing small amounts of lithium, including Li-ion, lithium polymer, and lithium cobalt oxide chemistries. Lithium-ion batteries containing more than 25 grams (0.88 oz) equivalent lithium content (ELC) are forbidden in US air travel.
Replacement batteries may be transported in carry-on luggage. Tips are provided on safe packaging and carriage of batteries; e.g., such batteries should be in their original protective packaging or in individual containers or plastic bags.
Some postal administrations restrict air shipping (including EMS) of lithium and lithium-ion batteries, either separately or installed in equipment. Such restrictions apply in Hong Kong, Australia and Japan.
On 16 May 2012 the United States Postal Service (USPS) banned shipping anything containing a lithium battery to an overseas address, after fires from transport of batteries. This restriction made it difficult to send anything containing lithium batteries to military personnel overseas, as the USPS was the only method of shipment to these addresses; the ban was lifted on 15 November 2012.
Researchers are working to improve the research methods, power density, safety, cycle durability, recharge time, cost, flexibility and other characteristics of these batteries.
Solid-state design (no electrolyte)
Solid-state lithium-ion batteries designs have the potential to deliver three times the energy density of typical 2011 lithium-ion batteries at less than half the cost per kilowatt-hour. This approach eliminates binders, separators and liquid electrolytes. By eliminating these, "you can get around 95% of the theoretical energy density of the active materials." Solid-state designs do not overheat or catch fire like traditional lithium-ion batteries can. They are much safer because they do not use liquid electrolyte. Plans are to have products ready for field testing as early as March 2015. Solid-state lithium-ion batteries are probably going to become the standard for electronics that are capable of operating in multiples of 3.2, 3.6 and 3.7 volts, respectively.
Washington State University researchers developed a tin negative electrode technology that they predicted would triple the energy capacity of lithium ion batteries. The technology involves using standard electroplating process to create tin nanoneedles that do not shortciruit when the tin expands by one third during charging.
Microporous tin has been used as a substrate for negative and positive electrodes that exhibit high energy density, power and fast recharge. The substrate self-assembles. Small spheres are packed onto a surface, forming a lattice. The area between the spheres is coated with the substrate material (nickel). The spheres are dissolved/melted and the resulting surface is electro-polished to enlarge the pores. Finally the substrate is coated with a thin film of the active material (Ni/Sn for negative electrode, LiMnO
2 for positive).
Higher lithium content electrode
Researchers at Amprius have created a lithium-ion battery that holds 20% more energy than the standard lithium-ion battery and they are in the process of producing higher levels of energy density. Theoretically, they can create a battery that can contain up to ten times as much energy density. They are using a silicon anode, rather than standard graphite (carbon). These new batteries are being produced with all the same materials as the standard.
Pomegranate style electrode for silicon anode
Researchers have discovered that using a pomegranate-inspired electrode with a silicon anode can reduce swelling while charging and reduce the gunk from the reaction with the electrolyte. This technique involves gathering yolk shells into clusters and then applying another coat of carbon around the cluster.
Researchers have previously overcome these problems by using silicon nanoparticles, which are already too small to break. They place the silicon nanoparticles in yolk shells made from carbon, with enough spare room inside for them to swell and shrink without causing damage.
Researchers have developed a battery that blends silicon and carbon that has a dramatic energy density improvement and five times the life cycle improvement than regular silicon anode lithium-ion batteries. The new silicon-anode batteries will allow electric vehicles to go 200–300 miles on a single charge. They are also cost effective and can be produced large scale.
Sticky liquid electrolyte
Researchers have developed a chewing gum like substance to replace liquid electrolytes. This new material contain liquid electrolyte but is sticky and thus eliminates the fire hazard. This material is also flexible so it can be used with bendable electronics in the future.
Disorder in battery materials
Creating lithium-ion batteries with disorder in the materials they are composed of has achieved 660 watt-hours per kilogram at 2.5 volts, a result rarely observed even in perfectly structured devices. Lithium-ion batteries are most commonly made of meticulously arranged rigid patterns of materials.
Researchers have discovered a way to make li-ion batteries flexible, bendable, twistable and crunchable using the Miura fold. This discovery comes on the heels of using all the same material of conventional lio-ion batteries and could be commercialized for foldable smartphones and other applications.
Nonflammable perfluoropolyether electrolyte
Researchers found a way to replace the electrolyte’s flammable organic solvent with nonflammable perfluoropolyether (PFPE), which eliminate the fire hazard. PFPE is usually used as an industrial lubricant. Researchers had originally been looking at using PFPE on the bottom of ships to prevent marine life from sticking, which is a serious problem in the world of shipping. More testing to see if the nonflammable electrolyte can withstand the rigors of everyday use, but they also exhibit unprecedented high transference numbers and low electrochemical polarization, indicative of longer battery life.
Germanium nanowire-based anode
Researchers have found that germanium nanowire-based anodes more than double the capacity of standard graphite anodes while still retaining high capacity even after being charged and discharged over 1,000 times.
Uniformity of li-ions into and out of cathode
Researchers have discovered a way to raise the charge durability to last four times more than traditional lithium-ion batteries while still maintaining adequate capacity. The process used maintains the lithium-ion diffusion at optimal levels and eliminates concentration polarization and thus allows the Li-ions to be more uniformly extracted from or reinserted into the cathode materials. This maintains the SEI layer at a stable state and prevents battery capacity fading.
Some of the companies interested in this new technology are concerned that this would mean fewer products are sold because the batteries would last so long. This lack of interest in bringing new technology is part of a corporate eco-system that holds technology back.
Architecture and controlling algorithm
Researchers have discovered a way to store 10-40% more capacity (specific energy of 110 – 175 Wh/kg) using their special battery pack architecture and controlling algorithm that allows it to fully utilize the active materials in battery cells.
Lithium iron phosphate cathode
Scientists at Massachusetts Institute of Technology have created Nanoball batteries that are capable re-charging 100 times faster than traditional li-ion batteries. They are capable of a 10 second re-charge in the size of a cell phone battery and a 5 minute re-charge in the size of an electric car battery. The cathode portion of the battery is composed of nanosized balls of lithium iron phosphate and the batteries can be charged much faster because the li-ion nanoballs transmit electrons to the surface of the cathode at a much higher rate. The batteries have also shown higher energy density and cycle durability than traditional li-ions. The issue is that the batteries also discharge at the much faster rate.
Single-walled carbon nanotubes
Researchers at Northwestern University have made discoveries about Single-walled carbon nanotubes (SWCNTs) that could help boost their energy density and cycle durability. They found that metallic SWCNTs accommodate lithium much more efficiently than their semiconducting counterparts. Another important discovery was that, if made denser, the semiconducting SWCNT films also begin to take up lithium at levels comparable to metallic SWCNTs. The team is also looking into other nanomaterials for research.
Analysis of cathode
Researchers at Nissan have developed a way to observe electrode material in the cathode during charging and discharging. This type of analysis could lead to higher energy density and higher cycle durability.
- Potassium-ion battery
- Nanowire battery
- Solid-state lithium-ion battery
- List of battery sizes
- List of battery types
- List of energy densities
- "Rechargeable Li-Ion OEM Battery Products". Panasonic.com. Archived from the original on April 13, 2010. Retrieved 23 April 2010.
- "Panasonic Develops New Higher-Capacity 18650 Li-Ion Cells; Application of Silicon-based Alloy in Anode". greencarcongress.com. Retrieved 31 January 2011.
- Valøen, Lars Ole and Shoesmith, Mark I. (2007). The effect of PHEV and HEV duty cycles on battery and battery pack performance (PDF). 2007 Plug-in Highway Electric Vehicle Conference: Proceedings. Retrieved 11 June 2010.
- Abe, H.; Murai, T.; Zaghib, K. (1999). "Vapor-grown carbon fiber anode for cylindrical lithium ion rechargeable batteries". Journal of Power Sources 77 (2): 110. doi:10.1016/S0378-7753(98)00158-X.
- Battery Types and Characteristics for HEV ThermoAnalytics, Inc., 2007. Retrieved 11 June 2010.
- Tsuyoshi Sasaki, Yoshio Ukyo & Petr Novák (14 April 2013). "Memory effect in a lithium-ion battery". nature.com.
- Ballon, Massie Santos (14 October 2008). "Electrovaya, Tata Motors to make electric Indica". cleantech.com. Cleantech Group. Archived from the original on 2011-05-09. Retrieved 11 June 2010.
- "Explain how lithium batteries work in electric golf carts". LithiumBoost. Retrieved 2013-05-09.
- Millsaps, C. (2012, Jul 10). Second Edition of IEC 62133: The Standard for Secondary Cells and Batteries Containing Alkaline or Other Non-Acid Electrolytes is in its Final Review Cycle. Retrieved from Battery Power Online (2014, Jan 10)
- Whittingham, M. S. (1976). "Electrical Energy Storage and Intercalation Chemistry". Science 192 (4244): 1126–1127. doi:10.1126/science.192.4244.1126. PMID 17748676.
- Besenhard, J.O. and Fritz, H.P. (1974). "Cathodic Reduction of Graphite in Organic Solutions of Alkali and NR4+ Salts". J. Electroanal. Chem. 53 (2): 329. doi:10.1016/S0022-0728(74)80146-4.
- Besenhard, J. O. (1976). "The electrochemical preparation and properties of ionic alkali metal-and NR4-graphite intercalation compounds in organic electrolytes". Carbon 14 (2): 111–115. doi:10.1016/0008-6223(76)90119-6.
- Schöllhorn, R.; Kuhlmann, R.; Besenhard, J. O. (1976). "Topotactic redox reactions and ion exchange of layered MoO3 bronzes". Materials Research Bulletin 11: 83. doi:10.1016/0025-5408(76)90218-X.
- Besenhard, J. O.; Schöllhorn, R. (1976). "The discharge reaction mechanism of the MoO3 electrode in organic electrolytes". Journal of Power Sources 1 (3): 267. doi:10.1016/0378-7753(76)81004-X.
- Besenhard, J. O.; Eichinger, G. (1976). "High energy density lithium cells". Journal of Electroanalytical Chemistry and Interfacial Electrochemistry 68: 1. doi:10.1016/S0022-0728(76)80298-7.
- Eichinger, G.; Besenhard, J. O. (1976). "High energy density lithium cells". Journal of Electroanalytical Chemistry and Interfacial Electrochemistry 72: 1. doi:10.1016/S0022-0728(76)80072-1.
- "USPTO search for inventions by "Goodenough, John"". Patft.uspto.gov. Retrieved 8 October 2011.
- Zanini, M.; Basu, S.; Fischer, J. E. (1978). "Alternate synthesis and reflectivity spectrum of stage 1 lithium—graphite intercalation compound". Carbon 16 (3): 211. doi:10.1016/0008-6223(78)90026-X.
- Basu, S.; Zeller, C.; Flanders, P. J.; Fuerst, C. D.; Johnson, W. D.; Fischer, J. E. (1979). "Synthesis and properties of lithium-graphite intercalation compounds". Materials Science and Engineering 38 (3): 275. doi:10.1016/0025-5416(79)90132-0.
- US 4304825, Basu; Samar, "Rechargeable battery", issued 8 December 1981, assigned to Bell Telephone Laboratories
- International Meeting on Lithium Batteries, Rome, 27–29 April 1982, C.L.U.P. Ed. Milan, Abstract #23
- Yazami, R.; Touzain, P. (1983). "A reversible graphite-lithium negative electrode for electrochemical generators". Journal of Power Sources 9 (3): 365. doi:10.1016/0378-7753(83)87040-2.
- Thackeray, M. M.; David, W. I. F.; Bruce, P. G.; Goodenough, J. B. (1983). "Lithium insertion into manganese spinels". Materials Research Bulletin 18 (4): 461. doi:10.1016/0025-5408(83)90138-1.
- Nazri, Gholamabbas and Pistoia, Gianfranco (2004). Lithium batteries: science and Technology. Springer. ISBN 1402076282.
- Voelcker, John (September 2007). Lithium Batteries Take to the Road. IEEE Spectrum. Retrieved 15 June 2010.
- US 4668595, Yoshino; Akira, "Secondary Battery", issued 10 May 1985, assigned to Asahi Kasei
- Manthiram, A.; Goodenough, J. B. (1989). "Lithium insertion into Fe2(SO4)3 frameworks". Journal of Power Sources 26 (3–4): 403. doi:10.1016/0378-7753(89)80153-3.
- Padhi, A. K. (1997). "Phospho-olivines as Positive-Electrode Materials for Rechargeable Lithium Batteries". Journal of the Electrochemical Society 144 (4): 1188–1110. doi:10.1149/1.1837571.
- "In search of the perfect battery" (PDF). The Economist. 6 March 2008. Archived from the original on 25 September 2009. Retrieved 11 May 2010.
- Monthly battery sales statistics. Machinery statistics released by the Ministry of Economy, Trade and Industry, March 2011.
- "Lithium Ion Battery Pioneers Receive Draper Prize, Engineering’s Top Honor", University of Texas, Jan. 6, 2014
- "At long last, new lithium battery tech actually arrives on the market (and might already be in your smartphone)". ExtremeTech. Retrieved 2014-02-16.
- Silberberg, M. (2006). Chemistry: The Molecular Nature of Matter and Change, 4th Ed. New York (NY): McGraw-Hill Education. p. 935, ISBN 0077216504.
- Thackeray, M. M.; Thomas, J. O.; Whittingham, M. S. (2011). "Science and Applications of Mixed Conductors for Lithium Batteries". MRS Bulletin 25 (3): 39. doi:10.1557/mrs2000.17.
- MSDS: National Power Corp Lithium Ion Batteries (PDF). tek.com; Tektronix Inc., 7 May 2004. Retrieved 11 June 2010.
- "How to rebuild a Li-Ion battery pack". Electronics Lab. Retrieved 6 June 2013.
- "Inside a notebook battery pack". ZDNet. Rupert Goodwins . August 17, 2006. Retrieved 6 June 2013.
- Andrea 2010, p. 2.
- Andrea 2010, p. 234.
- Wang, Y.; He, P.; Zhou, H. (2012). "Li-Redox Flow Batteries Based on Hybrid Electrolytes: At the Cross Road between Li-ion and Redox Flow Batteries". Advanced Energy Materials 2 (7): 770. doi:10.1002/aenm.201200100.
- Lithium Ion technical handbook (PDF). Gold Peak Industries Ltd. November 2003. Archived from the original on 2007-10-07.
- Choi, H. C.; Jung, Y. M.; Noda, I.; Kim, S. B. (2003). "A Study of the Mechanism of the Electrochemical Reaction of Lithium with CoO by Two-Dimensional Soft X-ray Absorption Spectroscopy (2D XAS), 2D Raman, and 2D Heterospectral XAS−Raman Correlation Analysis". The Journal of Physical Chemistry B 107 (24): 5806. doi:10.1021/jp030438w.
- Amatucci, G. G. (1996). "CoO2, the End Member of the LixCoO2 Solid Solution". Journal of the Electrochemical Society 143 (3): 1114–1110. doi:10.1149/1.1836594.
- Wenige, Niemann, et al. (30 May 1998). Liquid Electrolyte Systems for Advanced Lithium Batteries (PDF). cheric.org; Chemical Engineering Research Information Center(KR). Retrieved 11 June 2010.
- Balbuena, P.B., Wang, Y.X. (eds) (2004). Lithium Ion Batteries: Solid Electrolyte Interphase, Imperial College Press, London, ISBN 1860943624.
- Fong, R. A. (1990). "Studies of Lithium Intercalation into Carbons Using Nonaqueous Electrochemical Cells". Journal of the Electrochemical Society 137 (7): 2009–2010. doi:10.1149/1.2086855.
- Syzdek, J. A.; Borkowska, R.; Perzyna, K.; Tarascon, J. M.; Wieczorek, W. A. A. (2007). "Novel composite polymeric electrolytes with surface-modified inorganic fillers". Journal of Power Sources 173 (2): 712. doi:10.1016/j.jpowsour.2007.05.061.
- Syzdek, J. A.; Armand, M.; Marcinek, M.; Zalewska, A.; Żukowska, G. Y.; Wieczorek, W. A. A. (2010). "Detailed studies on the fillers modification and their influence on composite, poly(oxyethylene)-based polymeric electrolytes". Electrochimica Acta 55 (4): 1314. doi:10.1016/j.electacta.2009.04.025.
- Reiter, J.; Nádherná, M.; Dominko, R. (2012). "Graphite and LiCo1/3Mn1/3Ni1/3O2 electrodes with piperidinium ionic liquid and lithium bis(fluorosulfonyl)imide for Li-ion batteries". Journal of Power Sources 205: 402. doi:10.1016/j.jpowsour.2012.01.003.
- David Linden, Thomas B. Reddy (ed) (2002 ). Handbook of Batteries 3rd Edition. McGraw-Hill, New York, chapter 35, ISBN 0-07-135978-8.
- "Design Review For: Advanced Electric Vehicle Battery Charger, ECE 445 Senior Design Project". 090521 courses.ece.illinois.edu
- "Lithium Ion Rechargeable Batteries. Technical Handbook".
- M. C. Smart, L. D. Whitcanack and B. V. Ratnakumar. "Safe Charge Rates for Lithium-Ion Cells Effects of Lithium Plating". NASA Aerospace Battery Workshop. National Aeronautics and Space Administration (NASA). Retrieved 16 December 2013.
- Siemens CL75 user manual. Siemens AG. 2005. p. 8.
- Fisher, Thomas. "Will Tesla Alone Double Global Demand For Its Battery Cells? (Page 2)". Greencarreports.com. Retrieved 2014-02-16.
- "Reduced cell cost suggests the upcoming era of large capacity cells". EnergyTrend. 2013-05-06. Retrieved 2014-02-16.
- "Overview of lithium ion batteries". Panasonic. Jan 2007. Archived from the original on Nov 7, 2011.
- Winter & Brodd 2004, p. 4258
- "High Power Lithium Ion ANR26650M1A". a123systems.com. Archived from the original on 2010-06-01.
- Andrea 2010, p. 12.
- AeroVironment achieves electric vehicle fast-charge milestone avinc.com; AeroVironment, 30 May 2007. (Press release). "Test rapidly recharges a battery pack designed for use in passenger vehicles. 10-minute recharge restores enough energy to run electric vehicle for two hours at 60 miles per hour."
- "Imara Corporation website". Imaracorp.com. Retrieved 8 October 2011.
- O'Dell, John (17 December 2008). Fledgling Battery Company Says Its Technology Boosts Hybrid Battery Performance Green Car Advisor; Edmunds Inc. Retrieved 11 June 2010.
- Jost, Kevin [ed.] (October 2006). Tech Briefs: CPI takes new direction on Li-ion batteries (PDF). aeionline.org; Automotive Engineering Online.
- Loveday, Eric (23 April 2010). "Hitachi develops new manganese cathode, could double life of li-ion batteries". Retrieved 11 June 2010.
- Nikkei (29 November 2009). Report: Nissan On Track with Nickel Manganese Cobalt Li-ion Cell for Deployment in 2015 Green Car Congress (blog). Retrieved 11 June 2010.
- EnerDel Technical Presentation (PDF). EnerDel Corporation. 29 October 2007..
- Elder, Robert and Zehr, Dan (16 February 2006). Valence sued over UT patent Austin American-Statesman (courtesy Bickle & Brewer Law Firm)..
- Bulkeley, William M. (26 November 2005). "New Type of Battery Offers Voltage Aplenty, at a Premium". The Day. p. E6.
- A123Systems (2 November 2005). A123Systems Launches New Higher-Power, Faster Recharging Li-Ion Battery Systems Green Car Congress; A123Systems (Press release). Retrieved 11 May 2010.
- Garling, Caleb (20 April 2012). "IBM Demos Uber Battery That 'Breathes' | Wired Enterprise". Wired.com. Retrieved 22 June 2012.
- "... Acceptance of the First Grid-Scale, Battery Energy Storage System" (Press release). Altair Nanotechnologies. 21 November 2008. Retrieved 8 October 2009.
- Ozols, Marty (11 November 2009). Altair Nanotechnologies Power Partner – The Military. Systemagicmotives (personal webpage)[dubious ]. Retrieved 11 June 2010.
- Gotcher, Alan J. (29 November 2006). "Altair EDTA Presentation". Altairnano.com. Archived from the original on 2007-06-16.
- Synthetic Carbon Negative electrode Boosts Battery Capacity 30 Percent | MIT Technology Review. Technologyreview.com (2 April 2013). Retrieved on 16 April 2013.
- Newman, Jared (2013-05-23). "Amprius Begins Shipping a Better Smartphone Battery | TIME.com". Techland.time.com. Retrieved 2013-06-04.
- Andrea 2010, p. 229.
- GR-3150-CORE, Generic Requirements for Secondary Non-Aqueous Lithium Batteries.
- Sanyo: Overview of Lithium Ion Batteries, listing self-discharge rate of 2%/mo
- Sanyo: Harding energy specification, listing self-discharge rate of 0.3%/mo
- Zimmerman, A. H. (2004). "Self-discharge losses in lithium-ion cells". IEEE Aerospace and Electronic Systems Magazine 19 (2): 19. doi:10.1109/MAES.2004.1269687.
- Phil Weicker (1 November 2013). A Systems Approach to Lithium-Ion Battery Management. Artech House. p. 214. ISBN 978-1-60807-659-8.
- Winter & Brodd 2004, p. 4259
- Apple: Lithium-ion Batteries
- "Five tips for extending lithium-ion battery life". TechRepublic. Retrieved 14 February 2013.
- Specification sheet for typical lithium-ion battery
- Untersuchungen von Polarisationseffekte an Lithium-Ionen-Batterien In: Promotion Dr. Marcel Wilka 19. Dezember 2013.
- Andrea 2010, p. 9.
- Cristo, L.M. and Atwater, T. B. Characteristics and Behavior of 1M LiPF6 1EC:1DMC Electrolyte at Low Temperatures. Fort Monmouth, NJ: U.S. Army Research.
- "Modelling capacity fade in Lithium-ion cells, Bor Yann Liaw, Jungst, Nagasubramanian, and Doughty, Sandia National Laborator – Analysis of Lithium-Ion Battery Degradation during Thermal Aging" (PDF). Retrieved 8 October 2011.
- Tip: Condition your new cell phone’s battery to make it last longer (but be sure to condition it properly). Dottech.org (24 December 2011). Retrieved on 16 April 2013.
- Yadav, Antriksh. (31 December 2010) Top 5 lithium-ion battery myths. Rightnowintech.com. Retrieved on 16 April 2013.
- Spotnitz, R.; Franklin, J. (2003). "Abuse behavior of high-power, lithium-ion cells". Journal of Power Sources 113: 81. doi:10.1016/S0378-7753(02)00488-3.
- "Lithium-ion Battery Charging Basics". PowerStream Technologies. Retrieved 4 December 2010.
- Winter & Brodd 2004, p. 4259.
- Electrochem Commercial Power (9 September 2006). "Safety and handling guidelines for Electrochem Lithium Batteries" (PDF). http://marine.rutgers.edu. Rutgers University. Retrieved 21 May 2009.
- Mikolajczak, Celina; Kahn, Michael; White, Kevin and Long, Richard Thomas (July 2011). "Lithium-Ion Batteries Hazard and Use Assessment". Fire Protection Research Foundation. pp. 76, 90, 102. Retrieved 27 January 2013.
- Cringely, Robert X. (1 September 2006). "Safety Last". The New York Times. Retrieved 14 April 2010.
- "Can anything tame the battery flames?". Cnet . Michael Kanellos. August 15, 2006. Retrieved 14 June 2013.
- Guardian newspaper: Heathrow fire on Boeing Dreamliner 'started in battery component', 18 July 2013
- "Boeing 787 aircraft grounded after battery problem in Japan". BBC News. January 14, 2014. Retrieved January 16, 2014.
- "Are lithium batteries sustainable to the environment?". Alternative Energy Resources. Vaishnovi Kamyamkhane. Retrieved 3 June 2013.
- "Study Identifies Environmental and Health Impacts of Lithium-ion Batteries for EVs". May 28, 2013. Greenfleet Magazine. Retrieved 3 June 2013.
- "Can Nanotech Improve Li-ion Battery Performance". May 30, 2013. Environmental Leader. Retrieved 3 June 2013.
- "Kyocera Launches Precautionary Battery Recall, Pursues Supplier of Counterfeit Batteries" (Press release). Kyocera Wireless. 28 October 2004. Archived from the original on 7 January 2006. Retrieved 15 June 2010.
- Tullo, Alex (21 August 2006). "Dell Recalls Lithium Batteries". Chemical and Engineering News 84 (34): 11. doi:10.1021/cen-v084n034.p011a.
- Hales, Paul (21 June 2006). Dell laptop explodes at Japanese conference. The Inquirer. Retrieved 15 June 2010.
- Nokia issues BL-5C battery warning, offers replacement. Wikinews. 14 August 2007. Retrieved 8 October 2009.
- Nokia N91 cell phone explodes, Mukamo – Filipino News (27 July 2007). Retrieved 15 June 2010.
- "Safe Travel". Safetravel.dot.gov. U.S. Department of Transportation. 1 January 2008. Retrieved 8 October 2009.
- Galbraith, Rob (3 January 2008). "U.S. Department of Transportation revises lithium battery rules press release". Little Guy Media. Retrieved 11 May 2009.
- Prohibitions – 6.3.12 – Dangerous, offensive and indecent articles (PDF). Hong Kong Post Office Guide. December 2009. Retrieved 15 June 2010.
- International Mail > FAQs > Goods/Services: Shipping a Laptop. Japan Post Service Co. Ltd. Retrieved 15 June 2010.
- USPS To Stop Delivering iPads And Kindles To Troops And Overseas Consumers On 16 May. USPS. Retrieved 27 June 2012.
- Just in Time for the Holidays, U.S. Postal Service to Begin Global Shipping of Packages with Lithium Batteries USPS. Retrieved 6 December 2012.
- "Lithium ion cells for Aerospace applications: LVP series". GS UASA. Retrieved 17 January 2013.
- Dalløkken, Per Erlien (17 January 2013). "Her er Dreamliner-problemet" (in Norway). Teknisk Ukeblad. Retrieved 17 January 2013.
- Timmer, John. (2 August 2011) Retrieved 3 November 2011. Arstechnica.com. Retrieved on 16 April 2013.
- Melody Voth (6 December 2010). "Battery Booster". Chemical & Engineering News 88 (49). Retrieved 9 February 2011. (subscription required)
- Solid-state battery developed at CU-Boulder could double the range of electric cars, University of Boulder Colorado News, 18 September 2013
- WSU Researchers Create Super Lithium-ion Battery Retrieved 2013 January 10
- "Washington State University Gets Funding to Scale Up New Tin Batteries". MacroCurrent. 2013-04-30. Retrieved 2013-06-04.
- "Batteries charge very quickly and retain capacity, thanks to new structure | News Bureau | University of Illinois". News.illinois.edu. 2011-03-21. Retrieved 2013-04-20.
- "Small in size, big on power: New microbatteries a boost for electronics | News Bureau | University of Illinois". News.illinois.edu. 2013-04-16. Retrieved 2013-04-20.
- Nissan develops world first analysis technique for better lithium ion battery durability, Automotive World, 13 March 2014
- Amprius Gets $30M Boost for Silicon-Based Lithium-Ion Batteries, Greentech Efficiency, 6 January 2014, Jeff St. John
- At long last, new lithium battery tech actually arrives on the market (and might already be in your smartphone), Extreme Tech, 10 January 2014, Sebastian Anthony
- Pomegranate-inspired electrode could mean longer lithium-ion battery life, Gizmag, 19 February 2014, Nick Lavars
- EnerG2 Announces Major Breakthrough in Lithium-Ion Battery Capacity and Performance, PRWeb, 23 January 2014
- Chewing gum-like material makes lithium ion batteries safer, Tree Hugger, 5 February 2014, Megan Treacy
- Messy Innards Make for a Better Lithium Ion Battery, Scientific American, 17 January 2014, Umair Irfan and ClimateWire
- Origami: The surprisingly simple secret to creating flexible, high-power lithium-ion batteries, Extreme Tech, 5 February 2014, Sebastian Anthony
- First nonflammable lithium-ion battery will stop your smartphone, car, and plane from exploding, Extreme Tech, 13 February 2014, Sebastian Anthony
- Researchers Make Breakthrough in Battery Technology with New Tin-Seeded Germanium Nanowire Anode, World Industrial Reporter, 11 February 2014
- New tin-seeded germanium nanowire array anodes for Li-ion batteries show high capacity and lifetime, Green Car Congress, 10 February 2014
- New battery management technology could boost Li-ion capacity by 40%, quadruple recharging cycles, TreeHugger, 5 February 2014, Derek Markham
- New battery management technology could boost Li-ion capacity by 40%, quadruple recharging cycles, TreeHugger, 5 February 2014, Derek Markham
- Re-engineered battery material could lead to rapid recharging of many devices, MIT News, 11 March 2009, Elizabeth A. Thomson
- Zyga, Lisa (12 March 2009). "Nanoball Batteries Could Charge Electric Cars in 5 Minutes". PhysOrg. Retrieved 21 March 2012.
- Nanotubes make for better lithium-ion batteries, Nanotechweb.org, 3 March 2014
- Nissan develops world first analysis technique for better lithium ion battery durability, Automotive World, 13 March 2014
- Winter, M.; Brodd, J. (2004). "What Are Batteries, Fuel Cells, and Supercapacitors?". Chemical Review (PDFdoi:10.1021/cr020730k. PMID 15669155.) 104 (10): 4245.
- Andrea, Davide (2010). Battery Management Systems for Large Lithium-Ion Battery Packs. Artech House. p. 234. ISBN 1608071049. Retrieved 2013-06-03.
|Wikimedia Commons has media related to Lithium-ion batteries.|
- Lithium batteries at DMOZ
- Addressing the Impact of Temperature Extremes on Large Format Li-ion Batteries for Vehicle Applications, National Renewable Energy Laboratory, March 2013.
- Application of Life-Cycle Assessment to Nanoscale Technology: Lithium-ion Batteries for Electric Vehicles, U.S. Environmental Protection Agency, April 2013.